From Ingot to Target: A Cast Bullet Guide for Handgunners
Glen E. Fryxell and Robert L. Applegate
Foreword by John Taffin
From Ingot to Target: A Cast Bullet Guide for Handgunners A joint effort by Glen E. Fryxell and Robert L. Applegate
Foreword by John Taffin
About the Authors . . . Pg 5 Acknowledgements . . . Pg 7 A Few Words about Safety . . . Pg 9
Chapters 1. Introduction: A Brief History of Bullet Casting . . . Pg 11 2. Bullet Casting 101 . . . Pg 19 3. Alloy Selection and Metallurgy . . . Pg 27 4. Fluxing the Melt . . . Pg 37 5. Cast Bullet Lubrication . . . Pg 41 6. Throat and Groove Dimensions . . . Pg 56 7. Leading . . . Pg 58 8. Idle Musings of a Greybeard Caster . . . Pg 66 9. Moulds and Mould Design . . . Pg 73 10. Gas-checked vs. Plain-based Bullets . . . Pg 87 11. The Wadcutter . . . Pg 97 12. The Keith SWC . . . Pg 106 13. Casting Hollow Point Bullets . . . Pg 118 14. Making Cast HP moulds . . . Pg 131 15. Hunting with Cast Bullets . . . Pg 136 16. A Few of our favorites . . . Pg 148 Appendix A: How old is your mould? . . . Pg 173
Above: Left to right MP Molds Clone of the RCBS 45 caliber 270 Gr. SAA
SAECO #382 35 caliber 150 Gr. PB SWC SAECO #068 45 caliber 200 Gr.
SAECO #264 6.5mm 140 Gr. SP GC On the cover: Two RCBS 44 Caliber 300 Gr. Flat Point Mould Halves. One Mould was converted to Cramer style HP by Erik Ohlen with gas check shank removed from one cavity, casting one HP GC and one HP PB. Second mould casting both cavities flat point, one plain base, one gas check. Two moulds, four cavities, four different styles of hunting bullets. This book is copy right protected (copyright 2011). All rights are reserved by the authors. No part may be copied, reproduced or transmitted in any fashion without written permission of the authors.
Cover and index page photography by Rick Kelter Published exclusively at www.lasc.us
Foreword: by John Taffin
In many ways it seemed like only yesterday I began casting bullets. In fact it has been nearly one-half century since I started pouring that first batch of molten alloy into a single cavity mould, or mold if you prefer. It was in my mother's kitchen, at my mother's stove, next to my mother's refrigerator. It wasn't long before the whole top half of the side of her refrigerator was covered with speckles of lead. Now my mother was the most fastidious of housekeepers, however she never complained. Looking back I can only assume she thought it better to have me making a mess in her kitchen rather than running around doing something of which she didn't improve. At the time I was working for a large wholesale warehouse catering to plumbing and building contractors. This gave me access to both 100# bars of lead and one pound bars of tin. There was also a reciprocal agreement with a few other businesses allowing employees from one place to purchase from the other at wholesale prices. From the now long gone Buckeye Cycle I was able to order two Lyman single cavity molds, #454190 for the .45 Colt and #358311 for the .38 Special; a Lyman #310 Nutcracker Reloading tools with the dies for both .45 Colt and .357 Magnum, and I was ready to cast bullets. Those two molds are gone as it wasnt long before I graduated to multiple cavity moulds; however, I still use that #310 tool to pop primers from cartridges cases fired with black powder. Living as we do in the Instant Information Age, it is sometimes difficult to believe how little information was available or how difficult it was to find in the middle of the 20th century. I had read Elmer Keiths Sixgun Cartridges and Loads which gave me the very basics. Much of the rest I learned over the next four decades by trial and error and casting and shooting thousands upon thousands of cast bullets in hundreds of sixguns. Casting bullets opened all kinds of doors for me. Most importantly, casting allowed the shooting of vast amounts that would never have been had I found it necessary to buy my bullets from other sources. The only way to become even reasonably adequate with a sixgun is by shooting a lot, and only casting my own bullets allowed this. All of my shooting experiences, the vast majority of which has been with home cast bullets eventually led to my position as Field Editor with American Handgunner and Senior Field Editor with Guns magazines. Along the way, I not only managed to acquire a pretty good knowledge of cast bullets but also a working collection of approximately 250 bullet moulds from virtually every manufacturer. With this background in mind I now turn to the volume you hold in your hands. Glen Fryxell is a chemist by trade and a bullet caster by choice. He knows more about casting bullets than anyone else I know. Rob Applegate is both an excellent gunsmith as well as a maker of custom bullet moulds. Put the two of them together, and virtually every aspect of cast bullets is covered in what comes the closest to ever being called The Complete Book of Cast Bullets. Only their modesty prevents them from using this title and instead of going with From Ingot to Target: A Cast Bullet Guide for Handgunners. I found two things of major importance as I read this book. 1) The things
I've learned about cast bullets and casting bullets are true. 2) There was still much I needed to learn. Both what I know and what I needed to know are found in this book. Any well-informed sixgunner, even if they never intend to cast their own bullets, will find information here that simply make shooting more enjoyable. Which is better, plain-based or gas checked bullets? Why do soft bullets shoot well while hard bullets lead the barrel, and vice versa? How does bullet lube work? What is this mysterious thing called flux? How important are cylinder throat and barrel dimensions? Do cast hollow point bullets really work? Can one hunt with cast bullets, and if so which ones work the best? As important to me as the how-to information is the historical background. Over the years many men have contributed to our knowledge of bullets in general and cast bullets in particular. In these pages you will find such cast bullet pioneers as Elmer Keith, Phil Sharpe, Jim Harvey, Ray Thompson, Veral Smith, and my dear friend, J.D. Jones. Understanding their contributions simply makes shooting sixguns all that more enjoyable. If you have never cast a bullet but are planning to start, read this book first. Keep it at hand, and refer to it often. If you are an experienced bullet caster, stop; do not cast another bullet until you have read this book. You might be surprised at how much you have to learn. Rob and Glen have done an admirable job of gathering and presenting valuable information on what many think is a somewhat mystical or magical art. The doors are open, the lights are on, and the magic and mystery have been dispelled. This volume is a most valuable addition to both my loading room and my library. I expect all other dedicated sixgunners to also find this to be true. John Taffin Boise, Idaho
About the authors: Glen Fryxell has been fascinated with guns and hunting his entire life, and started hunting early, primarily with a bow and arrow during his teen years, and more recently with handguns. He obtained his B.Sc. in chemistry from the University of Texas at Austin in 1982, and his Ph.D. in chemistry from the University of North Carolina in 1986. Professionally, his interests have centered around environmental chemistry, nanostructured materials, molecular self-assembly and biomimetic processes. On the personal side, he is a hunter, shooter, reloader, and guitar player (of marginal ability). He has been casting bullets and reloading since the 1980s, and has hunted primarily with handguns over the last 20 years, taking dozens of head of big game and thousands of varmints, over much of the western US. His fascination with the use and performance of cast bullets in the hunting fields, in conjunction with his technical background in materials science and chemistry, led him to study the fascinating field of metallurgy in his spare time in an effort to more deeply understand bullet performance in the hunting fields. Rob Applegate was born with an innate passion to explore anything mechanical. If it moved, or had moving parts, he could not resist the temptation to dismantle all of the various parts in their entirety and find the causes of all the various movements and the forces behind the movements. In short, he was fixated on levers, grooves and pressures. The keen interest he had in mechanics manifested itself with firearms. As a little boy, he sat in stillness and watched with awe as his father patiently dismantled his sporting weapons and carefully cleaned and oiled each part before reassembling the rifle, revolver or shotgun upon which he was plying his gifted skills. This interest continued throughout all of his young life and beyond high school. His post high school education was centered around learning as much as possible about mechanics and eventually led to further education as to all of the various methods used to make the parts necessary to assemble machines of all types. After twenty five years of working "under the time clock", the opportunity presented itself for Rob to become a full-time gun maker. Being an avid shooter and tireless experimenter, Rob eventually became interested in casting bullets for a couple of old rifles passed down through the family to his dad. Bullets for the .40-82 Winchester were not readily available back in the late '50s and '60s, so Rob decided to he would make his own from the Winchester mould that was with the old '86. At that time, all that Rob knew about casting bullets was that "you melt lead in an iron pot, poured it into a mould, and after it cooled you opened the mould and out fell a bullet". Ahem, to say that he had much to learn is an understatement! But learn he did. As time passed, his skills and knowledge about casting bullets improved, along with this skills and knowledge about machining and tool-making. Most of his work as a custom gun-maker centered around single-shot and lever-action rifles, as well as revolvers. Nearly all of his barrel jobs and related work was for firearms that were dedicated solely for shooting cast bullets.
Whether they were black powder cartridge rifles, or the highest quality cast bullet bench rest rifles, the majority were to be used shooting cast bullets. All of the work on rifles and revolvers eventually led to the culmination of a dream and desire that Rob had had since childhood -- to make a bullet mould. Once he had refined mould-making to his satisfaction, he decided to make moulds on a full-time basis. For a number of years he made mould cherries and bullet moulds. During these mould-making years he learned more about bullet design than he thought possible. Eventually, several personal crises befell him, and the shop had to be closed. With most of these tragedies behind him, he would like to share some of his knowledge with the bullet casting fraternity.
With Glen Fryxell's excellent help in all aspects of the entire bullet casting science, we have compiled a work that is hoped will provide assistance to those who desire to shoot cast bullets in handguns. Glen is one of Rob's closest friends.
Acknowledgements: I am a student of the gun; or perhaps more accurately, I am a student of the bullet. I learn something every time I cast, load or shoot. Such an education clearly did not take place in a vacuum. I have the unwavering support of my lovely wife (who is still the nicest person I have ever met), a couple of great kids, and the most wonderful grandkids in the world (OK, so Im a little biased!). My parents have always been loving and supportive teachers, who valued education (and paid for much of mine), ensuring that I would have the ability to be a good provider. The resulting career has provided me with the wherewithal (and occasionally enough free time) to pursue those things that have fascinated me since early childhood; guns, hunting, bullet casting and handloading ammunition. Building upon that foundation are the contributions of a multitude of teachers, who have taught me these things, as well as gunsmithing, metallurgy, machine work and the art of integrating all of these disciplines in the pursuit of my own personal vision of ballistic perfection. The list of such teachers is far too long for any sophomoric attempt at complete-ness, but there are several men that I have been privileged to call friend whose guidance and insights must be acknowledged; Colonel Loveless of Pleasant Acres (College Station, Texas), who taught me marksmanship and ethics as a part of the NRA Junior Marksmanship Program when I was growing up back in central Texas; Dale Harber, who adopted me as a kid brother and took me hunting and nurtured my fascination with guns and handloading; Reo Rake, who got me started handloading and taught me the joys of the lead pot; Lyle Eckman, who taught me much, including how to shoot, listen and teach (once again, as a part of the NRA Junior Marksmanship Program); Dave Ewer, who is patiently teaching me the art of gunsmithing, and has helped me rediscover the joy of plinking; and John Taffin, for his guidance, advice and encouragement, for contributing to this book and for being a shining example of what a gentleman and gun-writer should be. Each one of these men is a crack shot, seasoned competitor, knowledgeable handloader and darned fine man. Thank you gentlemen. Lastly, I would like to thank Rob Applegate for being the ideal partner to write this book with. Rob is the kind of man that is met all too rarely these days, unfortunately. He is a hard-working, good Christian man. He is honest and industrious not just because he was taught that was the right way for a man to handle himself, but because he simply cannot operate any other way. It is his fundamental nature. He is a quiet gentleman, usually of few words, but when he speaks I listen, because Rob is a goldmine of knowledge on all things ballistic (among other things). Rob is the kind of friend that you can walk for miles through the mountains with and never say a word, because nothing needs to be said -- the mountains, wildlife, wind and clouds speak volumes, and he hasnt the rudeness to interrupt. Hes the kind of man that can be caught a mile and a half from the truck in his shirt sleeves in a surprise rainstorm and in conversation during the soggy walk back never once complain about the weather. Hes a giddy little boy who can spend hours out in his shop talking about the vice he made to cut mould blocks with, and while hes justifiably proud of his gadget, his real joy comes from the fact that his skills have created the ability to build new things, and to build them right. Much of Robs life revolves around building things. My Mother taught me many years ago, Any
fool can destroy. It takes a real man to build. Rob is a real man, a man who builds. He is a meticulous craftsman whose attention to detail is exquisitely apparent from the exceptional quality of his work. His nickname is Persnickety, and for good reason. Rob, we live too far apart. We should get together more often; you and Marilyn are special people. Thanks for everything, my friend. This book is a partial summation of these educational gifts, my primary contribution being my fascination with the subject and my unquenched desire to learn (and shoot) more. If the reader finds this book enlightening, educational or in some way of value, it is simply a reflection that I have been blessed with so many good teachers. Any flaws in the presentation are clearly my own. Glen Fryxell Kennewick, Washington Without Glen, this book would most likely have never happened in its completeness of text on the subject of casting bullets for handguns. His education in the sciences put a finality to the quandary about how and why alloys perform (or don't perform), both in the mould and in the bore. Glen is one of a handful of friends I have who looks past my stubbornness and basic anti-social behavior to have many deep discussions about cast bullet use and performance. To the men who were responsible for my education and training (my father, Uncle Rex, great-Uncle Gus Perot, etc.), I have said thank you and farewell, for they have all passed from this earth, as I will one day also. I have a few of the dearest friends anyone could hope for. To them I owe many thanks, not only for their encouragement for me to keep writing, but in many other things as well. For anyone who learns anything from this book, or who receives much needed help of advice, you can thank my lovely wife Marilyn for sorting out my hand-written scribbling and putting it all into an intelligible type-written manuscript. Without her, none of this would be possible. Each and every day, I thank God for the wonderful life I've had and for his Son, Jesus, the Great Forgiver. Robert L. Applegate Prineville, Oregon
A few words about safety OK, lets get one thing straight right from the beginning: casting bullets from molten lead can be dangerous. So can handloading ammunition, shooting a gun, driving a car, or operating power tools. However, if one thinks about the hazards associated with each of these practices, recognizes what and where they are, applies a little common sense, follows established safe practices and takes appropriate preventative precautions, the risks can be mitigated to the point that bullet casting is pretty much as safe as collecting butterflies. If you choose to cut corners, ignore safety rules, be lackadaisical or just flat dont think about what youre doing, you will get burned, and you may well poison yourself and those around you. Just like handloading, bullet casting is as safe or as dangerous as you make it. Bullet casting inherently involves hot metal, both the molten alloy that we fashion bullets from and the hot moulds and lead pots. Leather gloves are a good idea (and remember, a hot mould looks just like a cold mould, this is why we put wooden handles on them!). Even very small splashes of molten lead can cause nasty burns and leather does wonders for preventing them. And lead pots do splash -- when adding metal, stirring in flux, or if (heaven forbid!) they encounter any moisture. Keep all sources of moisture well away from your lead pot! A single drop of water can empty a 10 pound lead pot explosively, coating everything in the immediate vicinity with molten lead. If your lead pot is out on an open work bench, even minor splashes mean that safety glasses are a must. I cast with my lead pot wholly enclosed in a laboratory grade fume hood, with a glass sash in place between my face and the lead pot. I leave the little lead splatters in place on the glass sash as a reminder to myself as to how easily these things happen, and for instructional purposes for any new casters that I may be teaching. Good ventilation is very important to the bullet caster. My fume hood also serves to provide suitable ventilation, not only for the smoke coming off the pot but also for the heavy metal fumes emanating from the pot. Lead fumes are an obvious concern, but more subtle is the fact that wheel-weight alloy also contains small amounts of arsenic. Arsenic is kind of a quirk in the periodic table in that it forms an oxide that is more volatile than the metal, and in fact at lead pot temperatures, some forms of arsenic oxide are fully gaseous, so if the arsenic gets oxidized all of it evaporates from the lead pot and is easily inhaled. Use of a reducing cover material helps to prevent this oxidation (see chapter on fluxing). Fumes are not the only exposure vector that we need to be aware of, teething children like to put anything small and chewable into their mouths, especially if its bright and shiny. This includes cast bullets and discarded sprues, making housekeeping an important issue if small children have access to your casting area. This is easily dealt with, keep the sprues contained (heck just recycle them!) and keep the bullets packaged and out of reach of small fingers. Big fingers are an issue too: wash your hands thoroughly after each and every casting session, and again before you eat. Weve all heard about lead poisoning, but what does it really look like?
The symptoms of lead poisoning in adults include: loss of appetite, a metallic taste in the mouth, constipation, pallor, malaise, weakness, insomnia, headache, irritability, muscle and joint pain, tremors and colic. Lead poisoning can cause elevated blood pressure, sterility, and birth defects. The most significant site of lead toxicity is the central nervous system, but lead poisoning also impacts the red blood cells and chronic exposure to lead most often results in kidney problems. A childs body is more efficient at absorbing and retaining lead than is an adults, and lead gets stored in a childs growing bones. The net result is that children are far more vulnerable to lead poisoning than are adults, and since their central nervous systems are still growing and developing, the impact of lead poisoning on a childs life can be far more severe than it might be for an adult, and may include brain damage, mental retardation, convulsions and coma. Responsible handling of lead can prevent these exposures, symptoms and health hazards. Remember, safety first. Think about what you are doing, take appropriate precautions, use adequate ventilation, and keep your lead out of reach of small children. Bullet casting is a wonderful hobby and one that will allow you to get so much more out of your shooting, but just like handloading, bullet casting is only as safe (or as dangerous) as you make it.
Chapter 1: Introduction A Brief History of Bullet Casting: American Independence
Bullet casting contributed significantly to the independence of the western cowboy, trapper and mountain man. That independence is still valuable today. Just like the mountain man, once the modern caster buys a particular mould he can produce that bullet for the rest of his life, and he doesnt have to worry about whether commercial bullet makers will alter or drop a particular favorite from their line. The ability to produce countless thousands of identical bullets for decades to come reveals what a miniscule investment a bullet mould really is. History Originally bullet moulds were made and sold by the firearms manu-facturers themselves. Colt was an early player in the mould manufacturing game, making ball and conical bullet moulds for their early cap-n-ball revolvers. Shortly after the advent of the self-contained centerfire (i.e. reloadable) cartridge more sophisticated reloading tools became available. Soon after S&W graduated from rimfire cartridges to their centerfire Number 3 .44 American in 1870, they also added loading tools, including bullet moulds, to their product line. In the Remington catalogs of the 1870s are listed bullet moulds made by the Bridgeport Gun Implement Co. (BGI was a partner company, started around 1870 specifically to make loading tools for Remington). Winchester started making iron-handled bullet moulds in 1875 (and in a humanitarian gesture added wooden handles in 1890). In their 1876 catalog, Sharps advertised bullet moulds to make paper-patched bullets for their popular and powerful rifles. Marlin (Ballard) was also making moulds in the 1870s, and in 1881 enlisted none other than John M. Brownings input for a mould/loading tool that he designed and patented, and was subsequently manufactured by Marlin. The Maynard 1873 cartridge had a 5-piece case, very thick cartridge head and Berdan primer. The Maynard loading tools had a bullet mould, as well as a hook and a chisel for prying the spent primers out of the spent cartridge case. One of the more unique moulds from this era is that for the Maynard exploding bullet, a HP designed to be fitted with a .22 blank cartridge, advertised in the 1885 Maynard catalog in .40, .44 and .50 caliber. The 1870s were indeed a time of great change in the firearms industry. In 1884 John H. Barlow took his experience as a shooter and as a tool and die maker and founded the Ideal Company, offering his patented tong tools to reload spent cases, and later separate bullet moulds for those using bench-mounted presses. These bullet moulds were either single cavity, or 6- or 7-cavity Armory moulds, all with fixed handles at this point. The landscape was changing dramatically in the firearms industry in the late 1800s and early 1900s, and John Barlow kept pace with his contributions. His Ideal Handbooks (first published in the 1880's) were the first reloading guides published in America, of critical importance as shooters moved into the relatively uncharted territory of the then new smokeless powders. In Ideal Handbook #4 (published in 1890), he described the use of cast hollow-pointed bullets for enhanced performance on game animals. In Ideal Handbook #9 (1897) he unveiled the now familiar mould numbering scheme for Ideal's first 150 mould designs. In 1906, Barlow patented the first American gas-checked
cast bullet designs to take advantage of the higher velocities available from the new smokeless powders (described later that year in Ideal Handbook #17). In May of 1910, after leading the Ideal Manufacturing Co. for 26 years, Mr. Barlow retired and sold the company to The Marlin Firearms Co., with whom he had worked closely for many years. Marlin sold Ideal a few years later during the first World War to Phineas Talcott (but Marlin remained involved with production of the Ideal Handbook). By 1925 things were not going well and Phineas Talcott sold the struggling Ideal Reloading Tool Company to the Lyman Gun Sight Corporation (founded by William Lyman in 1878), along with the rights to the Ideal Handbook (which was later renamed The Lyman Handbook with #27, published in 1926). Lyman scaled up manufacturing capacity and continued production of the Ideal line of bullets moulds, using the Ideal name into the late 1950s. During this time Lyman introduced interchangeable mould blocks in their single cavity moulds (first advertised in the American Rifleman in 1927, and cataloged in 1931), and phased out the older fixed handle style. In 1940-1 (Ideal Handbook #34), Lyman added a special retaining pin to hold their hollow point plug in place during casting. Interchangeable double cavity mould blocks didnt appear until after World War II (first listed in the Ideal Handbook #36, which was published in 1949), followed soon thereafter by venting lines cut in the faces of the mould blocks. Interchangeable 4-cavity mould blocks were introduced in 1958. Lyman continues to produce many of these mould designs to this day.
Note the lack of alignment pins and the hand-
cut vent lines.
Early Ideal rifle bullets were designed not only by John Barlow, but also by such notable shooters as Harry Pope, Col. Townsend Whelen, and Phil Sharpe, among others. In the early 1920s, a vociferous northwestern cowboy, rancher and competitive shooter named Elmer Keith went to Belding & Mull with some of his
ideas for experimental revolver bullets. Belding & Mull made the moulds (interestingly, B&M moulds were made out of solid nickel) and Keith assembled and evaluated many test loads using these bullets. Keith learned much from these experiments with cast bullet design, but he never quite got to where he wanted to be. In 1928, shortly after Lyman bought the Ideal Co., he turned to Lyman and asked them to make some bullet moulds according to his optimized designs. Thus was born the Keith SWC. The Keith SWC's have 3 equal width driving bands, a square-cut grease groove, a beveled crimp groove, a sharp wad-cutting shoulder, a compound-radiused ogive for stable long-range flight, and a healthy, meat-crushing meplat. They have proven themselves over the last three quarters of a century as some of the finest revolver bullets of all
An Ideal Armory mould for the 360344 wadcutter.
time. The original Keith SWC was for his beloved .44 Special (#429421), but Keith/Lyman went on to produce similar moulds in other calibers (e.g. .357, .45, etc.) and in hollow-base and hollow-point variations. Similar fixed handle moulds were also made by the Yankee Specialty Company. These were made out of bronze and were commonly cut with the same designs as used by Ideal, including the Keith SWC's. Yankee Specialty made 1, 2 and 3 cavity moulds, as well as HP moulds (they claimed to have over 600 designs available). Yankee Specialty was in business from 1916 until the owner died in 1954, although their business volume after 1940 was small. Yankee moulds are commonly unmarked and have simple cylindrical wooden handles that are wired on (although a few are reported to have ferrules). Things got busy on the American bullet casting scene in the second quarter of the 20th century. George Hensley was a machinist involved in the manufacture of all sorts of things (like bicycles, a gasoline fired marine engine, etc.), as well as doing general machine work and repair, with his company that he started in 1893. In 1932, he started turning out some top-notch moulds from his shop in San Diego in response to the demand for multiple cavity moulds needed by police departments. The P.D.'s had to supply practice ammunition for their officers and needed moulds capable of casting larger numbers of bullets than what was generally available at the time. The Great Depression meant that budgets were tight, and affordable practice ammo was
a significant need, just as it is today. James Gibbs was a farm boy from the Midwest who was very mechanically inclined and was operating a small gunsmithing shop on his own. James met up with George Hensley in the late 1930s as a result of their common interest in firearms, and Mr. Hensley quickly saw James talents and the two struck on an agreement for James to help George out in the shop making moulds. Hensley & Gibbs worked together from 1938 to 1940, when George became too old
to work in the shop. Eventually, he sold the business to James in 1950. The partnership of Hensley & Gibbs produced some of the finest moulds ever made, including 6, 8 and 10 cavity gang moulds that were the mainstay for many
A copy of the Ideal 452423, made by Yankee Specialty Co. with integral handles (Yankee
Specialty also made a few moulds with interchangeable blocks). This Depression-era
mould is made from bronze, not iron.
Police Departments and shooting clubs. Their reputation for quality was such that Elmer Keith went to H&G in the early 1960s to get them to re-introduce the original Keith SWC designs after Lyman had modified his design (much to his
A well-used Hensley & Gibbs 10-cavity #51BB .38 semi-wadcutter
mould (note the particularly massive sprue plate).
displeasure) by changing the width of the driving bands and going to a smaller, rounded grease groove. Keith was very pleased with the H&G products. Initially, H&G operated out of San Diego, but in 1964-1965 moved to Oregon's historic Applegate Valley, to the small town of Murphy. Wayne Gibbs eventually took over for his James (his father) and Wayne continued to run the family business until the mid-1990s. Hensley & Gibbs moulds are now available through Ballisti-Cast Manufacturing. Cramer Bullet Mould Co. (of North Hollywood, CA) started producing some very well-made cast-iron moulds sometime around 1937. They made 2, 3 and 5-cavity moulds, as well as the more typical 6, 8 and 10-cavity gang moulds. Cramer's 10-cavity gang moulds were constructed of a unique, patented design. There were two parallel rows of 5 cavities each, with 3 mould blocks (a center block, and the two outer blocks with handles mounted). The sprue plate, instead of swinging through an arc (as most do) was grooved such that it was struck to move down the long axis of the mould, away from the caster. Only after the sprue had been struck could the mould be opened. It was claimed that this enhanced production rate and efficiency. In December of 1951 Santa Anita Engineering Co. (better known as SAECO, who made lead-pots and lube-sizers in Pasadena, CA) took over production of the Cramer line of moulds, and focused mainly on 2 and 4-cavity moulds. In 1971, Saeco added 8-cavity gang moulds to their product line. In 1985, Saeco was bought out by Redding (the well-respected makers of precision reloading dies) and moved to Cortland, NY. Redding has made Saeco bullet moulds ever since. The 8-cavity bullet moulds were phased out in 2002.
Bond Manu-facturing Co. appears to have started in the mould-making business sometime around 1910. Shortly before WW I, they teamed up with Modern Equipment Corp., and officially changed the name to Modern-Bond shortly after the War to End All Wars. They made all manner of reloading tools, but especially bullet moulds. Modern-Bond appears to have closed up shop in1951. The Modern-Bond Corporation was the originator of the Inter-
Advertisement (circa 1939) of the unique Cramer 10-cavity gang
changeable block moulds which have been extensively copied by other manufacturers., so states the Modern-Bond ads appearing in the American Rifleman back as early as 1927 (in response to Lyman/Ideal's ad claiming to
have invented the concept). This was turf-staking claim was brought on when Lyman/Ideal started making Inter- changeable single-cavity mould blocks in
1927 (even though they weren't cataloged until 1931). Modern-Bond may have had some sort of patent protection on multiple cavity moulds with exchangeable blocks, which might explain why Lyman didnt produce such moulds until 1949 (although George Hensley certainly did in the 1930s). In any event, Modern-Bond turned out an extensive line of both rifle and pistol designs in well-made 2-cavity moulds during the 1920s up through about 1950. If a prospective customer wanted to examine a Modern-Bond bullet design in the
flesh they would send sample bullets through the mail for a nickel apiece.
A single-cavity Herter's .38/.357 SWC mould
cut by Lyman, with a 358156 cavity, with the Herter's sprue plate.
The Herters mail order catalog contained gear to outfit just about any flavor of outdoor adventure, from fly-fishing, to back-packing, to bow-hunting, to fur trapping. Included in this Nirvana of the Northwood's was an extensive selection of bullet moulds for the casting enthusiast. Generally, these mould designs and mould numbering scheme were
Picture of a Modern-Bond F-257-730 mould (a .25 caliber 86 grain GC-RN), showing the unique black lacquered handles
of the Modern-Bond moulds.
identical to Lyman's, revealing the origin of their mould blocks (which by the way are un-marked), although sometimes Herter's just labeled the mould with bullet diameter and weight. All of the Herter's moulds I've seen were single-cavity, but their catalogs listed double-cavity moulds as well. The Herter's sprue plates were slightly different than the Lyman sprue plates, having a small tab bent over the edge of the blocks to serve as a stop instead of the Lyman method of having a stop-pin mounted in the mould blocks. The sprue plate was also stamped with "HERTER'S INC. WASECA, MINN. U.S.A.", along with the mould design number, and the sprue plate pivot screw had no "keeper" screw. Herter's extensive selection of moulds included HP moulds for the .32-40 and .45-70 rifles, but the
A Cramer 5 cavity .38 wadcutter mould.
only pistol HP cataloged in 1969 was for the .32-20 (31133). A number of HB mould designs were cataloged for both rifles and pistols. The 1968 Gun Control Act seriously bit into Herter's business, and they eventually folded up shop. Used Herter's mould are still encountered today, albeit infrequently. Lachmiller of Glendale, California entered the loading tool business in 1952, and offered a complete line of reloading tools, dies, sizers, presses, etc. In 1969 Lachmiller introduced a line of well-made 2 and 3-cavity bullet moulds. Lachmiller continued to make bullet moulds into the 1970s, but then sold off their product line to RCBS in the later part of that decade.
Ohaus started offering bullet moulds in a big way in 1972, entering the market with 68 different bullet designs, as well as 19 round ball moulds. Ohaus moulds were cut with tungsten carbide cherries for durability and consistency. A few years later RCBS bought out Ohaus, and continues to produce many of these bullet moulds today. Lee entered the bullet mould market in 1973, offering inexpensive aluminum moulds that have allowed beginning casters to get started affordably. Their 6-cavity
pistol moulds (which were introduced in 1989) provide an affordable way to make a pile of pistol bullets in a hurry.
RCBS mould .40 caliber.
Stepping back and looking at the overall picture of bullet mould manufacture in America, we see production of bullet moulds shifting from the firearms manufacturers to stand-alone companies that made reloading tools from the 1880s through the early 1900s. This was followed by a flurry of activity in the middle half of the 20th century, especially in the post-war 40s and 50s. Then, through the course of
mergers, buy-outs, and closures we see the number of outfits making bullet moulds dropping off towards the end of the century. As the 20th century closed, there were 4 major manufacturing houses still producing bullet moulds; Lyman, RCBS, Saeco (Redding) and Lee. Of course, there were also a number of
A Lachmiller 3-cavity .38 SWC mould.
smaller shops offering specialty and custom mould making services, such as NEI, Hoch, LBT and Rapine. Sadly
however, great mould makers like Cramer, Lachmiller, and Modern-Bond are
Lee 6-cavity .45 ACP TC mould.
heard from no more. To cast with one of their rugged moulds is to relive history with sweat, smoke and vintage iron in your very hands. Why do we cast? Back in the days when Elmer Keith was drawing up 429421, a shooters need for bullet casting equipment was much more of a driver than it is for us today. Living on remote ranches in the Pacific Northwest in the 1920s, availability of reloading components was limited and mail-orders were slow and of spotty reliability. Keiths ministrations (as well as those of other gun-writers of the day) were well-received by the American shooting public and the popularity of casting grew in the 1940s and 50s to a kind of Golden Age of Bullet Casting, in which most serious handgunners had an assortment of moulds with which to feed their flock. In recent decades, this tendency has all but disappeared. Today, we have more manufacturers turning out a greater selection of higher quality components than ever before. High-volume businesses, with massive inventories, have sprung up to scratch most every conceivable shooters itch. As a result, in todays world of e-business, its no problem to rattle off an online order and have it accurately filled and on your doorstep in 24-48 hours. Times have changed, indeed! Given this Land of Milk and Honey why would anyone want to cast their own bullets? Why not just reap the advantages of cast bullets by shooting those available commercially? There are quite a few cast bullets available commercially, and virtually all of them have a Brinell hardness number (BHN) of 20 or greater, and are decorated with some mysterious flavor of gaily colored hard lube. We, as Americans, have a tendency towards the thinking that if a little is good, then more is better, so if Elmer Keiths beloved 429421s cast of 16-to-1 alloy had a BHN of 12 and were good, then a commercial hard-cast bullet with a BHN of 22 must be better, right? Nope, hard bullets certainly have their place, but they are generally not ideally-suited for routine revolver shooting (these reasons behind this will be developed in more detail in the alloy selection chapter). So why are commercial cast bullets so hard? Remember the bit about living in a world of overnight delivery? The reason that commercial casters make their bullets so hard is so they can withstand the rough and tumble conditions of shipping. What good are those lovely 429421s at a BHN of 12 if they show up on your doorstep, dinged, dented and out-of-round? Commercial cast bullets are cast that hard as a means of damage control, plain and simple. The home-caster has the freedom to cast bullets whatever hardness his specific load and gun require, without worrying what some unknown freighter is going to drop on them. Once again, the ability to cast one's own bullets provides independence from external worries. Commercial casters generally tend to cast only those bullets that are available for casting machines (e.g. Magma), in an effort to maximize their output. After all, their bottom-line is time equals bullets, and more bullets equal more money. Almost invariably, these machine moulds have rounded features, and are bevel-based (BB) to insure that the bullets release easily from the mould, thereby speeding up production rate. If you dont want one of these generic designs, or youre looking for a specific profile for a specific application, or if you dont like BB bullets, then youre pretty much stuck. On the bright side, there are a few shops that still cast from hand-held moulds and offer traditional PB designs like the Keith SWCs, etc. But remember, these are hand-
made bullets, not mass-produced from a casting machine, so you can expect to pay extra for their hand-crafted services. If you want designs that are even more time-consuming to cast, like traditional hollow-base bullets for some of the old black powder cartridges, or cast hollow-points for hard-hitting hunting loads, not only are these mould designs slow to cast and therefore more expensive to produce, but they are very poorly served by the hard alloys used by commercial casters (BHN of 20). Casting your own bullets provides the independence to produce these bullets at will, in your exact alloy of choice -- no worries, no waiting. Commercial bullet casting is a business, plain and simple, and the product line is going to be dictated by business volume. The commercial caster is going to sell a lot of .38 WCs, 9mm RNs and .45 SWCs, so thats what they are going to produce. Thats just good business sense! But what if you have a .40-50 Sharps Bottle-neck, or a .405 Winchester, or a .41 Long Colt, and need bullets of an unusual diameter and you dont feel like paying a buck apiece (or more) for custom jacketed bullets? Or you dont want to wear out a valuable old, soft barrel? The purchase and use of one bullet mould will keep you and your cherished piece of firearm history shooting for many, many years. Imagine being able to call up Hornady (or Nosler, or Sierra, or Speer) and saying, You know, I really like your .357 JHPs, but they dont expand quite the way I want in my favorite load. I need some with a core composition of 2% tin, no antimony. When can you have, say, 500 of them ready for me? Or, Your 250 grain .45 RNFP is a great bullet, but its .451 diameter and I need it made with a diameter of .454 for my old Colt SAA. How soon can I get a couple hundred? Obviously, a major commercial bullet manufacturer would go broke trying to satisfy such requests, but the shooter who casts his own bullets can make these adjustments easily, and have the results ready to shoot today. Once again, we return to the central theme of independence. With the resurging interest in cowboy action shooting and traditional guns and loads, once again shooters are turning to hot, smoky moulds to produce their projectiles. Partly for nostalgic reasons, partly for period authenticity, but also I think partly because the modern day shooter likes to feel that same independence that the cowboys and mountain men of the late 19th century felt. There is something very satisfying about making your own bullets. Yes, the hobby of bullet casting can fuel large volumes of inexpensive shooting; yes, cast bullets are gentler on the rifled bore; yes, it is a very satisfying hobby that allows the shooter to put more of themselves into their shooting and therefore to get more out of it; and yes, cast bullets allow some fine old guns to be shot that could not be shot otherwise, but in the end, bullet casting all boils down to independence. It provides the shooter with the ability to produce as many bullets of whatever diameter, whatever design, and what-ever composition, as they want, for the rest of their life. It is precisely this sort of self-reliant independence that made America strong. God bless America!
Chapter 2: Casting 101 Casting Basics
Shooters who cast their own bullets add a whole new dimension to their
handloading endeavors. As a bullet caster, you will open new doors to experimentation with ammunition and you will become your own bullet supplier. This chapter will deal with the physical details of casting bullets.
The old phrase the best place to start a task is at the beginning, is in a
way, humorous, but also very true in learning the techniques and the science involved in casting bullets. Safety of the bullet caster is of utmost concern to the authors and it is at this point that you are reminded to please study the chapter on safety before undertaking the melting or pouring of lead alloy. Assuming you have studied the chapter on safety, we will proceed to learn the art and science of casting your own lead alloy bullets. The chapters following this one will go into detail about the various bullet alloys, bullet hardness, bullet lubes, to gas check or not to gas check, and fluxing the alloy.
Cleanliness and purity in the alloy you use and a good clean mould are
paramount to making good bullets. Any volatile solvent, even in the form of vapor, will prevent complete fill-out in the cavity and no useable bullets can be made until the mould is completely free from any petroleum distillates or other solvents.
If you are a beginning caster and are starting with a brand new mould,
you may have a patience-taxing task ahead of you; please do not lose heart! Breaking in a new mould will net more than just a good casting mould; it will give you a life-long companion for your shooting activities. Mould break-in involves oxidizing the cavity interiors. This is accomplished first by pre-heating the mould on top of your melting pot (provided you have a large enough ledge on your pot to safely hold the mould with its handles), and second, by casting bullets in the mould. The time you spend pouring bullet alloy into the cavities of your new mould will give you experience in the techniques of pouring, controlling the alloy, learning how it reacts to temperature changes, and the effects that the pouring rate and temperature have on the quality of the bullet.
Working with good equipment will make it easier for you to learn the skill
of bullet casting. High quality expensive equipment is not mandatory for casting good bullets, although it certainly makes learning easier for the beginner and lessens the likelihood of frustration. As our good friend John Taffin likes to say, "Cheap equipment is too expensive!" Good tools make the job go easier, and will provide a lifetime of service.
Your first need in getting started will be a very well ventilated and dry
area in which to set-up your equipment. No water can be allowed to come in contact with the molten alloy. A fan may be necessary to move hot and contaminated air away from the casting area. It is best to situate the fan so the moving air flows over the top of the pot and does not blow directly on it.
A good quality melting pot will be your first large investment. Whether
the pot is a ladle pour or a bottom pour, it should have a temperature control
on it calibrated in degrees (although this calibration scale may not be all that accurate, it gives you a means of reproducing those conditions that work best for your particular equipment). If you choose a bottom pour pot, it should have a rugged, adjustable pouring valve. If you choose to use a separate heating source and melting pot, it will be necessary to purchase a casting thermometer so you can keep track of the alloy temperature (these are available from a variety of sources and commonly cost around $30).
Your next investment will be a mould suitable for the caliber you wish to
supply bullets for. Generally it is easier to cast bullets of .38 caliber or larger and of short, simple design. Learning the skills of obtaining good quality bullets will require much less effort and concentration on your part by starting out with a mould designed to cast bullets designed for handgun use. The beginning caster will learn how to regulate the flow of the alloy to achieve complete fill-out of the cavity for high quality, uniform bullets. You will become familiar with the feel of the mould/handle assembly in your hand as the alloy fills the cavity and the sprue countersink. Each type of cavity and each size of sprue hole have a particular flow rate and temperature where it produces the best results.
The next two purchases you make will be the alloy and flux you intend to
use. As mentioned earlier, separate chapters on fluxing and the properties of the various alloys follow this one and you will need to study those before doing any casting or making any purchases.
The next two items are ones you most likely already have. You need an
old towel folded up so the still hot and slightly soft bullets will have a soft surface to fall upon ejection from the mould. The other item is a hardwood stick or piece of 1 dowel about 12 14 long. The length and diameter are not critical as long as you are comfortable using it. This hardwood rod will be used to either push or tap open the sprue plate after making a cast in the mould. A piece of handle from a rake or hammer can work well for this purpose and may be something you already have in your garage or shop.
The last remaining item will be a scooper/stirrer you can use to stir in the
flux and scoop the sludge from the top of the melt. A wooden handle is very valuable here as this tool routinely gets very hot in use. Do NOT use aluminum or anything containing zinc in your alloy. Also do not use any kind of eating utensil, as it will be heavily contaminated with lead in use and might get mixed back in with the silverware, poisoning whomever eats with it.
Now that you have accumulated all of the necessary tools and equipment
and have studied the pertinent casting information in this book, you are ready to heat up the pot, warm the mould blocks which are assembled to their handles, and start pouring bullet alloy into your mould cavities.
Just a reminder before you start heating up the pot: REVIEW THE CHAPTER ON SAFETY FIRST!
Make sure the mould is completely clean. Alcohol can be used for a final
cleaning (and is good for removing petroleum distillates and other solvents). Most of the solvents used for electrical and automotive brake lining degreaser
work well for initial cleaning and removing preservatives and cutting oil residue left in the mould from the manufacturer.
Assuming you are using an electric melting pot, plug in the power supply
cord as per the manufacturers recommendation. Set the thermostat to about 750o. While the pot is warming with the ingots of clean bullet alloy resting inside the pot, place the complete mould on the ledge of the pot so the blocks themselves are actually on the ledge and NOT the wooden handles. This will allow the mould blocks to slowly preheat.
Once the alloy in the pot has melted, it will need to be fluxed, stirred,
and later skimmed of the dross (crud) that has floated to the top. After the fluxing operation is concluded, you are then ready to take hold of the wooden end of the mould handles and start filling the cavities with molten bullet alloy from the pot. If you are using a ladle, place the ladle over the pot and begin allowing it to heat, by very slowly lowering the ladle into the melted alloy. When fully submerged, leave the ladle head in the alloy for a couple of minutes to thoroughly heat soak it to the same temperature as the alloy. Go ahead and remove the ladle full of alloy and pour the alloy back into the pot using the pouring nozzle. Repeat this process a few times to get used to the feel of pouring through the nozzle and seeing how the alloy behaves while being poured. The lead alloy, when at the correct pouring temperature, will flow much like water or very thin oil. Now you are ready to pour lead alloy from the ladle into the mould cavities.
If you are right handed, it may be easier to hold the ladle in your right
hand and the mould in your left. Turn the mould top face (sprue plate) vertically so the sprue holes face to the right. Now place the ladle's pouring spout (or nozzle) up against one of the sprue plate holes with the ladle pouring nozzle firmly pressed to the sprue pouring hole, and turn both the mould and ladle together as a unit upright, thereby causing a portion of the alloy in the ladle to flow into and fill the bullet cavity in the mould. If you have a two-cavity mould, repeat this process with the second cavity. Place the ladle back in the pot. Wait a few seconds for the alloy in the sprue hole countersinks to solidify (this metal is commonly referred to as "the puddle"). With your wooden rod, push or knock the sprue plate open. Swing the plate fully open. Open the mould and let the bullets fall onto the soft towel you prepared. It may be necessary to tap the handle hinge to eject stubborn bullets. Repeat this whole pouring procedure as many times as needed until you are comfortable with the entire process. As you cast with the ladle you will see a dull looking sludge begin to build up on the ladle and inside the pot. This needs to be fluxed and stirred back into the melt. Now that you have some experience in pouring bullets, you can refine your technique by learning to pull the ladle back enough after the cavity is filled, to leave a puddle of alloy in the sprue countersink. Filling the countersink prevents voids in the bases and concave bases. Both conditions invite leading and inaccuracy caused from improperly filled-out bullet bases.
The process with bottom pour pots is essentially the same as with using a
ladle except that the alloy flows directly from the bottom of the pot through the nozzle. A valve to which the handle is attached controls the flow. The handle is mounted toward the front of the pot for easy access.
Some casters have trouble casting good bullets with a bottom pour pot. The only difference between the ladle method and bottom pour method is that the bottom pour pot has the entire vessel full of alloy sitting on top of the nozzle. This condition is generally termed head pressure. Only experience wrought through trial and error will teach you how best to adjust and regulate the flow of alloy on a bottom pour pot for complete fill-out with each design of mould cavity you cast bullets in. Normally, higher temperatures are required when using a bottom pour pot. It may be necessary for the pot temperature to be set as high as 850o. It is recommended that a layer of charcoal or sawdust be placed on top of the melt to protect it from oxidation. This subject is discussed in the fluxing chapter. Keeping the pot only half full may also help eliminate some of the fill-out problems and render the regulation of flow easier to adjust and less sensitive to the technique of the caster. Whether using a ladle or bottom pour casting, the flow of alloy into the cavities of the mould has to be sufficient in volume and pressure to adequately fill out the cavity. You may need to develop a technique of rocking the mould away from the pouring nozzle ever so slightly just as the cavity comes to near full. This allows any air to escape from the top of the cavity during the critical base fill-out phase and it makes it easier to leave a full size sprue puddle. It may be necessary to have a slight air gap between the sprue hole and the nozzle. The amount of gap will vary from one mould to the next and can only be determined by experiment-tation. Different moulds can have differing "tastes" in terms of how they "prefer" to be fed: some cast best with a half an inch of free fall for the alloy below the pour spout, whereas others (especially HP moulds) may perform best when "force-fed" (i.e. the mould held directly against the pour spout so the full force of the head pressure helps to force the alloy into the cavity). Recording the settings and adjustments for each mould may save you much set-up time in future casting sessions. Mould guides are available from the pot manufacturers for most of their bottom pour pots. Always fill the sprue plate countersinks with a puddle of alloy after the cavity is full to allow for any shrinkage as the bullet cools. Keep your pour constant and fill both the cavity and the sprue in one continuous smooth motion. Experience is the best teacher in learning these skills, and the more you do it, the better caster you will become.
Do not expect your first bullets to be shoot-able. You will be very
disappointed if you think your new mould will make perfect bullets the first time out. They WILL get progressively better with time (and practice), and soon you WILL be casting perfect bullets. Bullet casting is both fun and profitable because it is something you do for yourself. Relax and enjoy doing it and dont demand too much from yourself at first. As you progress further along with your casting practice you will notice that your bullets will improve in quality and appearance. This is due to the mould warming up and breaking in and improvements in your skills as a bullet caster. Under normal circumstances once a mould is broken in, it stays that way. Our learned skills and abilities are pretty much the same way. Once learned, they are not quickly forgotten.
Bullets that come from the mould wrinkled, not well filled out, are bright
and shiny indicate either a too cool mould or alloy or both. When bullets become frosted and possibly eject stubbornly from the mould, the mould itself is too hot. Moulds that have small cavities and large blocks may need to be placed on a warm hot plate until they begin casting properly. You may need to
do this occasionally throughout the casing session. Moulds with small blocks and large cavities may need to be set aside for brief periods to cool throughout the casting session. Advanced casters sometimes cast with two moulds alternating between the two to keep them at ideal operating temperatures. If the mould has a tendency to overheat, a fan can be located to blow on the mould while you are ejecting the bullets. NEVER, EVER, PUT YOUR MOULD IN WATER WHILE IT IS HOT! The mould will be warped beyond repair and steam and hot water may scald you.
Bullets with unfilled bases or air pockets may need a bigger sprue
puddle. If the bullets are frosted, you will need to cool the mould slightly and turn down the temperature setting on your pot to about 50o 100o. Bullets that show a cold mould condition will require the alloy temperature to be increased by 50o 100o and more casting with the mould to bring it up to efficient operating temperature.
The following paragraphs are a brief summary of what we have covered
in this chapter and can be used as a quick reference. 1. Safety is the primary concern when working with molten metal. A
ventilated workplace is mandatory. Make sure the type of ventilation method you choose, pulls the harmful vapors and hot air AWAY from you. Always dress yourself in suitable protective clothing, such as closed top work boots, leather apron, gloves, and face protection before the alloy melts. NO WATER should be allowed anywhere near the casting area. Water coming in contact with molten lead will cause a violent explosion.
2. Pre-heat the mould on the large ledge at the top of the pot. Cast bullets for awhile to finish warming the mould.
3. Shiny, wrinkled bullets indicate a cold mould. Keep casting bullets until the mould is up to temperature and/or turn up the pot temperature 50o to 100o.
4. Frosted bullets indicate a too hot mould. Allow the mould to cool for awhile and/or decrease the pot temperature 50o 100o.
5. Wrinkled, poorly fill-out bullets coming from a hot mould indicate petroleum distillate in the mould or on the sprue plate. If the mould was thoroughly cleaned before casting was begun, the heat from the alloy should eventually remove the petroleum vapors with further casting. This will be obvious if the quality of the bullets improves with further casting.
6. An adequate flow of lead has to be maintained while the cavity is filling and to also fill the sprue countersink. Alloy has to be forced into all areas of the cavity to make a fully formed bullet. Head pressure in bottom pour pots can only be regulated by the level of the lead in the pot. The flow is regulated by the adjustment at the handle that limits the amount that the valve is opened. Too much head pressure accompanied by overheated alloy can actually force lead into the cavity with such force that it causes bullets to stick in the cavity and will also cause fins on the bullet where the lead has flowed out into the vent lines. Sticking bullets will require using the wooden rod that you use to open the sprue plate with, to whack the hinge area of the
handles to jar the bullet loose from its stuck position in the cavity. If the alloy is at normal casting temperature and the bullets are not filling out, try either increasing or decreasing the rate of flow at the nozzle. And record your settings for future set-ups.
7. If the sprue plate swings back over any part of a bullet's base, it will prevent that bullet from falling freely from the cavity.
8. Drop the bullets from the mould onto a soft towel-like surface to prevent damage to the still hot and somewhat soft bullets.
9. SAFETY FIRST!
Before the bullets can be loaded and shot, they must be lubricated and sized. Several manufacturers of casting equipment offer excellent sizer lubricators. The basic lubrisizer unit is fitted for interchangeable sizing dies and nose punches. Study the chapter on determining the correct size bullet for your application. Once the correct bullet diameter has been determined and the die and nose punch has been acquired, you are ready to fill the lubrication reservoir and ready the device for use. Follow the manufacturer's directions for installing the die, nose punch, and filling the reservoir. For flat-nosed bullets, a universal nose punch can be used, which insures that the bullet will self-center in the sizer die. Some bullets require the use of a gas check. So long as the gas check shank of the bullet fits the gas check, the check can be placed on the shank with the fingers before placing the bullet on the plunger of the die. A separate section on annealing gas checks is included in Chapter 10. Once the lube-sizer is set-up and ready for operation, you are ready to set your first bullet on the sizing die, lower the operating handle and push the bullet down into the die. For the Lyman and RCBS style lube-sizers, turning the handle counter clockwise on the lube plunger screw pulls the lube plunger into the lube changer and forces lube through the holes in the die and into the lube grooves in the bullet. It may take several cycles of lubricating bullets to bleed all the air from the chamber and die. Air pockets in the lubricant chamber and die will result in incomplete filling of the lube grooves. On occasion, portions of lube grooves will not want to fill and will require cycling the bullet back into the die with lube pressure applied on the die to fill in the vacant area in the lube groove. It may not be necessary to tighten the screw any further if enough pressure is already applied. Most of the time, passing the bullet back through the die once will be adequate enough to fill the groove with lube. The die has holes drilled through it at intervals to allow the lubricant to pass from the chamber of the lube-sizer into the interior of the die. With handgun bullets it is a fairly easy matter to align the grease groove(s) in the bullet with the holes in the die by adjusting the depth stop located at the bottom of the lube-sizer. With most handgun bullet types when the grease groove in the bullet is aligned with the grease hole in the die, the groove will fill with grease on the first pass. Bullets with multiple grooves will have the grooves filled as the grooves pass by the holes in the die on the way down into the die and on the way back. Now that your first batch of bullets are lubricated, sized, and/or
gas-checked, the lube chamber plunger screw needs to be backed off about one full turn. This prevents grease from bleeding past the die plunger and from between the die body and lube-sizer bore. It also relieves pressure from the internal parts and body. Backing off the screw between uses is also important, if the tool is going to sit unused during seasonal changes where the weather passes from the cold of winter to the heat of summer. Bullet lube expands as it warms. As a result, excess pressure can build inside the tool and crack the housing of the pressure chamber ruining the tool. Heaters are available for your lubrisizer in the event that you want to use a hard lube that requires heat to flow properly. Always remember to back off the screw BEFORE using a lube heater. A light bulb placed near a cold tool can warm overly stiff grease so as to make it more fluid to better fill the bullet grooves. Pressure to the screw should only be applied AFTER the lube is fully warmed. If pressure is applied before or during the warming process, excessive pressure can build in the tool and crack the housing. During the lubricating process it will be necessary to maintain enough grease (lube) pressure to fill the grease grooves of the bullet and at the same time not to allow excessive pressure to build that will force lube between the die plunger and the bullet base. With combinations where the bullet is slightly smaller than the die lube will leak around the bullet. Other than being messy and wasting lube this is not a problem as long as the grease grooves are being filled. As in the skill of casting, lubricant pressure regulation will be learned through the experience of operating the tool. Some bullet designs have a smaller front driving band than the bullet body. With such designs it is essential that you do not allow the bullet to go too deeply into the die. If the undersized driving band of the bullet is allowed to pass below the lube holes in the die, lube will push out into the void and make a mess, which slows production and wastes lube. Moulds that are not made properly or are out of adjustment may cast slightly out of round bullets. For handgun use this is not generally a problem. The authors of this book have shot surprisingly tight groups from handguns shooting bullets up to .009" out of round. In some cases, no difference in group size was detected between groups shot with perfectly round bullets and these out of round bullets. In other cases, this asymmetry can make a tremendous difference. The only way to know for sure if out of round bullets will have an impact on your shooting, with your gun, is to shoot them and see (adjusting an out of round mould is addressed in more detail in the Idle Musings chapter). When sizing bullets that are slightly out of round, the only noticeable effect will be that of varying depths of crimp and lube grooves. One side will have normal depth grooves and the other side will have more shallow grooves and the variation in depths will depend on the amount the bullets are out of round. Occasionally, a lube-sizer will leave the factory with the bores for
the ram and die slightly offset from one another. If you happen to obtain one of these units, please do not attempt to repair it. Return it to the manufacturer for a replacement. It is easy to determine if the unit you are using has offset bores. The bullets you size, no matter how perfectly round they come from the mould, will always be sized heavier on one side than the other. Normally, lube-sizers are perfectly made and will last most folks an entire lifetime. The care you give your equipment both while using and in storing it will determine how well it performs and how long it will last. The modest investment of a bullet mould and a lead pot can provide you with a lifetime supply of bullets.
Chapter 3: Alloy Selection and Metallurgy Lead was one of the first metals that Man learned to purify and manipulate. There are lead figurines still in existence that date back to 3800 BC. Ancient Phoenician trade in lead is described in Ezekiel, XXVII, 12. The ancient Greeks, Romans and Hebrews also mined and worked lead long before the birth of Christ. It has been used for millennia, in a wide variety of applications. Lead-based plumbing (from the Latin name plumbium and hence its chemical symbol Pb) and lead containing pewter goblets and wine casks were thought to be one of the primary reasons for the downfall of ancient Rome. Lead-based solders made the graceful beauty of medieval stained glass windows possible. Chronic lead poisoning is now known to have killed the musical genius Ludwig von Beethoven (although the source of lead is still a mystery). The United States continues to be a leading producer of lead and it has been mined here since 1621, when the first North American lead mine and smelter were opened near Falling Creek, Virginia. Lead has played a central role in human history. Lead has been the principle ingredient of bullets for centuries, and its choice for this application is logical: it is dense, easily formed, and widely available. Back when projectiles were patched round balls, it wasnt necessary to alloy it with anything to make it harder or to get it cast well, because the surface tension of the molten lead made it want to go to a sphere anyway. But when bullets started taking on convoluted shapes and started getting stuffed into cartridge cases, then the limitations of pure lead surfaced. In order to get the molten alloy to properly fill out the ridges and grooves of the mould cavity it was necessary to add something to the lead to lower the surface tension. In addition, breech-loading cartridge rifles had arrived on the scene, and brought with them higher velocities that required harder bullets. Initially the answer to both of these problems was found in the addition of small amounts of other metals (e.g. tin) to harden the alloy moderately. To form a simple substitutional alloy, it is necessary that the added metal have a similar atomic size and electronegativity to the primary metal. Tin satisfies these requirements, mixes with lead very easily, significantly improves castability by lowering both viscosity and surface tension, and hardens the alloy moderately well. Everything was rosy, but then those confounded chemists started playing with nitrate esters of various organic materials and suddenly smokeless powder made its somewhat awkward, but spectacular entry. These new developments meant that much higher pressures and velocities were now possible. The cast bullet would need to get harder. Cast bullets have always been a natural fit for handguns. But keep in mind that the American handgunner of the first quarter of the 20th century was working with loads at less than 1000 fps for the most part. The .38 Colt Automatic and the .38-40 were the hot-rods of the day at roughly 1100 fps (the exception being the .30 Mauser, but there werent that many in the US during this time, and the .38 Super wouldnt appear until 1929). Men like Phil Sharpe, Major Wesson and Elmer Keith experimented with high pressure loads in some of the stronger guns of the day, but the .357 Magnum wasnt to see the light of day until 1935, and the .44 Magnum had to wait until 1956 to make its appearance. The handloading handgunner of the first quarter of the 20th
century was, for the most part, loading cast bullets at about 850 fps. The modest binary alloys of the black powder era (e.g. 20:1 to 30:1 range) were entirely adequate for this ballistic regime. Three things happened, slower pistol powders were developed (2400 came out in 1933), magnum revolver cartridges were invented, and tin got to be progressively more and more expensive. It was found that magnum handguns could be made to shoot well with cast bullets IF they were sufficiently hard (hard in this case being somewhere in the 10:1 to 16:1 range, with a Brinell Hardness Number, or BHN, of 11 to 12). One of the cast bullets desirable attributes is affordability, but if youre dumping a full pound of tin into every 10 pound pot of bullet metal, it can get expensive fast! Thus other solutions were sought for hardening bullet metal. Metallurgy of the Cast Bullet Lead-tin (Pb-Sn) - Which metals do we add to lead to make better bullet metal and why? The first and most obvious need here is to make the alloy harder, but there are other factors that play into this answer as well. Historically, tin was used because it was readily available in pure form, mixed easily with molten lead and contributed desirable properties to both the molten and solidified alloy (castability and hardness, respectively). Tin also increases the hardness of the alloy but does not interfere with the malleability of lead (a key point that well return to). Tin lowers the viscosity and surface tension of the molten alloy, allowing it to fill out the mould more effectively, resulting in a higher quality bullet. Tin is limited in its ability to harden lead, achieving a maximum hardness of about 16 BHN at 40% tin. These binary lead-tin alloys undergo slight to moderate age softening upon storage (1-2 BHN units), with the harder alloys undergoing more of a change than the softer alloys. The hardness of a binary lead-tin alloy generally stabilizes after about 2-3 weeks. Heat treating binary lead-tin alloys does not provide any change in hardness. At typical lead pot temperatures, lead and tin are infinitely miscible with one another, at the eutectic temperature (361o F) tin is still soluble to the tune of 19%, but at room temperature tin is still soluble in lead at the 2% level, meaning that as the bullet cools down there is significant precipitation of a tin-rich solid solution in the form of granules and needles in a matrix of lead-rich solid solution. It is important to recognize that tin is well-mixed in the matrix and it hardens lead by making the matrix itself harder.
Lead-antimony (Pb-Sb) - Antimony on the other hand hardens lead alloys much more efficiently, with only 1% antimony producing a BHN of 10 while it takes 5% tin to do the same, and it takes only 8% antimony to achieve a BHN of 16, as compared to 40% tin. The name antimonial lead refers to binary lead alloys with 1-6% antimony, with the higher antimony alloys (i.e. those with >1% antimony) commonly being called hard lead
in industry. While antimony increases the hardness of lead, it does so by
BHN of Binary Lead-Tin A
0 10 20 30 40 50
impairing its malleability. At typical lead-pot temperatures (ca. 700o F), antimony is only moderately soluble in lead alloys, and as the temperature drops, the solubility of antimony is markedly lower than that of tin. At the eutectic temperature for a binary lead-antimony alloy (484o F), only 3.5% antimony is soluble (note that this is 123o F hotter than of the tin eutectic temperature, but the antimony solubility is less than 1/5 that of tin). At room temperature the equilibrium solubility of antimony in lead is only 0.44%. The precipitated antimony appears as small rods, at the grain boundaries and within the grains themselves. Electron micrographs of lead-antimony alloys clearly show discrete particles of antimony surrounded by a matrix of lead-rich solid solution. In contrast to lead-tin alloys, lead-antimony alloys age harden, sometimes as much as 50% or more. When these alloys are air-cooled, some antimony is retained in the lead-rich matrix and as a result these alloys age-harden as this antimony continues to slowly precipitate. This usually takes 10-20 days to achieve full effect. It is important to recognize the antimony hardens lead alloys by a fundamentally different mechanism than does tin. Antimony hardens the alloy by precipitation of a separate crystalline antimony phase, which reinforces the
squishy plastic lead phase thats in between the hard antimony crystals. These alloys tend to be brittle because the plastic (squishy) lead phase gets its hardness from the reinforcing hard antimony rods. As the matrix gets deformed the brittle antimony rods shear off and the soft metal fails. In the case of the lead-tin alloys, the tin is more uniformly distributed through out the matrix, making the matrix itself harder, so plastic deformation of the
alloy is more uniform and progressive, not the slip/shear of lead-antimony alloys.
BHN of Binary Lead-Antimony Alloys
0 1 2 3 4 5 6 7 8
Multi-component alloys - Tin still improves castability by lowering viscosity and surface tension. Antimony hardens the alloy via precipitation. The tin also helps to alleviate brittleness by combining with the antimony to form an intermetallic adduct thereby improving the solubility, maintaining the hardness. Antimony also helps to reduce shrinkage as the alloy cools. The harder the alloy, the less it shrinks (lead shrinks 1.13%, linotype shrinks 0.65%). In molten lead alloys, tin and antimony react with one another to form an intermetallic compound (shorthand is SbSn to show the adduct between antimony, Sb, and tin, Sn). This does a number of things. First of all, SbSn is more soluble in lead than is Sb. In addition, both free Sb and Sn are soluble in SbSn, as is Pb, meaning that the formation of this phase serves to enhance the mixing of the alloy and limit phase segregation and precipitation. When Sb and Sn are present in roughly equal amounts, the alloy behaves as though its a pseudobinary system of SbSn in Pb. Electron micrographs of 94% Pb, 3% Sb and 3% Sn (an excellent bullet metal, very similar to WW alloys with 2% added tin) shows globular grains of lead rich solid solution, with an interdendritic
pseudobinary eutectic of SnSb phase (for example see: the Metals Handbook: Volume 7, Atlas of Microstructures of Industrial Alloys, page 304). Similar electron micrographs of linotype alloys show very thin dendrites of lead-rich solid solution, surrounded by a matrix of SnSb intermetallic phase, with much precipitated antimony rich solid solution (this precipitated phase is why linotype bullets are so brittle and tend to shear upon impact). How these alloys are hardened depends on the composition. The malleability of lead-tin-antimony tertiary alloys depends heavily on composition, particularly on the tin/antimony ratio. When the concentrations of tin and antimony are equal, the alloy behaves as though its a binary system with SnSb as the diluents in the lead matrix. The phase behavior of SnSb is notably different than that of Sb -- both in terms of solubility and in terms of crystal morphology. Sb is highly crystalline and only soluble in Pb to the tune of 0.44% at room temperature. SnSb appears to be significantly more soluble in Pb and based on electron micrographs of chemically etched samples, significantly more amorphous. As mentioned before, the SnSb phase serves as a mixing agent, serving to help dissolve excess Sb (or Sn for that matter), and having greater solubility in the Pb matrix. This enhanced mixing, along with the reduced crystallinity means that the lead alloys with a 1:1 ratio of tin to antimony behave somewhat like simple binary lead-tin alloys, only harder (this is why Lyman #2 is 90% Pb, 5% Sb, 5% Sn). Hold this thought As the concentration of antimony increases over that of tin, at first the SnSb phase serves to dissolve the small amount of excess Sb. At higher Sb concentrations however the SnSb phase becomes saturated and a separate antimony phase begins to precipitate. At this point, the alloy begins to take on some of the brittleness properties of the binary lead-antimony alloys. As the antimony concentration increases, this brittleness becomes more pronounced. So those tertiary alloys which have 2 or 3 times as much antimony as tin (e.g. linotype, 12% Sb, 4% Sn) tend to be more brittle than those alloys of similar hardness with similar Sb and Sn levels. OK, heres a subtle point, WW alloy (3% antimony, 0.3% tin) can fall prey to this issue as well, although not as severely since its not as hard. But by adding tin and making the alloy slightly harder, the alloy also becomes less brittle and more malleable due to the formation of SnSb and the elimination of the precipitated Sb phase. Thus, WW alloy with approximately 2% added tin makes an excellent bullet metal with hardness suitable for a variety of applications, and it still can be made harder through heat treating or water quenching. This can also be made using Lyman #2 mixed with an equal amount of pure lead.
Hardness of Tertiary Lead/Antimony/Tin Alloys Alloy Composition Hardness Lead - - - 5 Wheelweights 95% Pb, 3% Sb, 0.3% Sn, 0.2% As 12 Lyman #2 90% Pb, 5% Sb, 5% Sn 15 Linotype 84% Pb, 12% Sb, 4% Sn 22 Lead based Babbitt 85/10/5 19 Lead based Babbitt 80/15/5 20
In Cast Bullets by E. H. Harrison (NRA Publications) WW alloy +2% tin is listed as giving very good castability and a BHN of 13.6. My own measurements run more like a BHN of 11-12 (undoubtedly due to the variation in WW content), but this alloy does indeed cast very well. Recovered range scrap varies from range to range, depending on the nature of the shooting at that particular locale, but it commonly runs fairly soft (in the BHN range of 8 or so) as a result of all the .22 Long Rifle and swaged .38 wadcutter ammo deposited in with the jacketed and hardcast bullets. Age hardening of the tertiary alloys is more pronounced in the softer alloys, suggesting that at the higher antimony concentrations precipitation occurs more readily during the cooling process. This age hardening can be accelerated by increasing the aging temperature. In general, measuring bullet hardness 24-48 hours after casting provides the most useful and timely information.
Age Hardening of Tertiary Lead/Antimony/Tin Alloys (In BHN) Alloy As-cast 6h 48h 6 days 6 months Lead 5 No change
97/2/1 9.2 17.1 20.2 21.6 18.0 94/3/3 12.4 14.1 16.9 18.2 16.6 (electrotype) 82/12/ 20.3 20.3 20.1 19.9 17.7 (stereotype)
In addition, arsenic (As) is commonly added to industrial lead-tin-antimony alloys to improve the strength (this strength enhancement is only observed when As is added to a Sb containing alloy, As is virtually worthless in the absence of Sb). Arsenic also significantly enhances the ability of the alloy to be hardened via heat treatment. All that is needed is 0.1% (more does no good). Wheelweight alloy commonly contains about 0.17% As. Heat treating and water quenching - This age hardening of antimony containing alloys can be accelerated at higher temperatures, i.e. heat treating the bullets. This is most commonly done by sizing the bullets first (since lead alloys work soften, and hence sizing would negate a significant portion of the hardness imparted by the heat treating process) then heating them to about 450o F in the oven and quenching by dumping them in cold water. The hardened bullets are then lubed using the same sizing die that was used before (so that no actual sizing takes place). Done in this manner, bullets cast with an alloy containing 5% antimony, 0.5% tin and 0.17% arsenic, which would normally have a Brinell hardness of a little over 16 (after aging for 6 days), can be hardened to a BHN of over 35 (see Dennis Marshalls chapter Stronger Bullets with Less Alloying in Cast Bullets published by the NRA). Notice that this alloy is not tremendously different from the common wheelweight. Much the same sort of result can be obtained by casting with a hot mould and water quenching directly from the mould (place a towel over the water bucket with a 4 slot cut in it to contain the splashes). Mould temperature is critical for maximum effective hardness. Bullets water quenched from a cool mould (i.e. one from which the bullets were smooth and shiny) were found to be similar to air-cooled bullets. But bullets dropped from a mould that was hot (i.e. hot enough that the bullets were frosty over their entire surface) were found to have BHN of over 30 when water quenched. In a separate study, such a mould
was found to have temperature of 430o F, very similar to the optimum oven temperature found in the heat treatment study (ca. 450o F). I dont normally cast quite this hot, but even so, water-quenching WW alloy routinely gives me bullets with a Brinell hardness of 18. One of the advantages of hardening bullets in this manner, as opposed to using linotype to make them hard, is that they are tougher and not as likely to shear or fragment on impact. Why are we so worried about hardness? In the old days, there was a lot of talk about bullet hardness, and how soft bullets could cause leading by having the bullet metal getting scraped off as the overly soft bullet traversed the bore. But keep in mind, in the old days; they considered a pure lead bullet soft (with a BHN of 5) and a 16-to-1 bullet hard (with a hardness of 12 BHN). We cast with harder alloys today, and what is considered hard and soft today is very, very different than in pre-WWII America. The problem is, the Old-timers spoke in terms of hard and soft, not in terms of measured hardness values, so a new caster going back and reviewing the older casting literature is easily confused about what causes leading (addressed in detail in a later chapter). Commercial casters almost universally exploit this confusion and use it as a part of their sales pitch, touting their hard-cast bullets (commonly with a BHN of 18-22) as being the perfect remedy to prevent leading. Taint necessarily so, Compadre. Extra hard alloys can actually cause leading (again, see the chapter on leading for a detailed explanation of this). The bottom-line is if youre casting bullets for typical revolvers (standard and magnum, ignoring rounds like the 454 Casull, which is a case unto itself, see the chapter on GC bullets), and if you are using an alloy with a hardness of at least 11 BHN, any leading you observe is not caused by the alloy being too soft. Remember, Elmer Keith used the Lyman 429421 cast of 16-1 with a BHN of about 11 for the .44 Magnum. What is surprising is that today all these newcomers that get all hot and lathered worrying over whether their 20 BHN bullets are too soft!?! Obturation - OK, if we know that soft bullets with a BHN of 6 can cause problems, why dont we just cast everything out of linotype? If a little hardness is good, then more is obviously better, right? Well, aside from being a really expensive way to make cast bullets, there are some physical drawbacks to this approach. Obturation is the plastic deformation of the bullet metal in response to the applied pressure (from the burning powder). Cast bullet obturation was extensively studied and characterized by Dr. Franklin Mann over a century ago, and summarized in his most excellent treatise The Bullet's Flight from Powder to Target. Using soft cast bullets, he observed bullet swelling from several thousandths of an inch to several calibers, depending on the conditions employed (pressure, barrel condition, etc.). Modern barrels are exceptionally well-made, but there are minor imperfections (one or two ten-thousandths of an inch) in groove diameter, the width of the lands and grooves, minor local variations in twist rate, etc. As the bullet is engraved, these minute imperfections result in an imperfect seal bet